- Email: [email protected]

Contents lists available at ScienceDirect

Composite Structures journal homepage: www.elsevier.com/locate/compstruct

Numerical analysis of interlaminar stresses in open-hole laminates under compression A. Solisa, S. Sanchez-Saeza, X. Martinezb,c, E. Barbero-Pozueloa,

T

⁎

a

Department of Continuum Mechanics and Structural Analysis, University Carlos III of Madrid, Spain International Centre for Numerical Methods in Engineering (CIMNE), Spain c Department of Nautical Science and Engineering, Polytechnic University of Catalonia (UPC), Spain b

A R T I C LE I N FO

A B S T R A C T

Keywords: Open-hole Compression Interlaminar stresses Fibre microbuckling

In this paper, the interlaminar stresses in open-hole laminates subjected to compressive loads are analysed using a numerical model. This model implements the Serial/Parallel Mixing Theory (S/PMT) and a Continuum Damage Mechanics (CDM) approach. The S/PMT estimates the global stiﬀness in the laminate from ﬁbre and matrix properties. The CDM approach models the damage initiation due to ﬁbre microbuckling. The global response estimated by the model was veriﬁed with experimental data from the literature. The model predicts that the damage initiates in the laminate middle-plane where the thickest block of plies oriented in the load direction is located, and progressively propagates to the nearest block of layers with the same orientation. Two laminate stacking sequences were analysed. The interlaminar stresses around the hole presented symmetry with respect to the load direction and the perpendicular axis, being located the maximum and minimum values in diﬀerent angular positions for each stress component and laminate.

1. Introduction

signiﬁcantly lower than the tensile strength, in the order of 60% for many composites, and thus the damage initiate at lower stress [10]. In addition, the failure mechanisms under compressive and tensile loads are diﬀerent. There are several mechanisms that can contribute the laminate failure [13]. For example, under tensile loads, the ﬁbre failure is controlled by ﬁbre breakage, while in compression, the mechanism that produce the ﬁbre failure is the microbuckling [10,14,15]. The damage of laminate begins by ﬁbre microbuckling in sublaminate scaled laminates with plies at 0° [16,17] and can propagate by other failures modes such as matrix cracking and delamination [18,19]. The damage of laminates with ply at 0° (sublaminate level scaling) begins by ﬁbre microbuckling [16,17] and can propagate by other failures modes such as matrix cracking and delamination [18,19]. Many works can be found in the scientiﬁc literature on modelling of in-plane stresses and damage evolution around a hole in a laminate subjected to tensile [20-23] and compressive loads [9,10,16,24]. In spite of these works, there is a necessity to continuous working in the knowledge of the problem of open-hole laminates subjected to compressive loads. Several methodologies can be applied to study laminates containing holes subjected to diﬀerent load states. The simplest models only can predict the ﬁnal failure [25-27]. More complex models can predict damage initiation and growth [23,28-35]

Structural components usually have notches and holes that produce a phenomenon of in-plane stress concentration that could reduce their strength signiﬁcantly. In addition, interlaminar stresses appear in these components close to the free-edges, even when in-plane loads are applied. These stresses can be relevant and contribute to the laminate failure due to the low interlaminar strength of composite laminates [1]. Interlaminar stresses control two damage modes, shear failure and delamination. The shear interlaminar stresses can produce matrix crack at the free-edge, and the normal stress in the thickness direction contribute to generate damage by delamination [2,3]. The analysis of the interlaminar stresses at the free-edge in laminates has been studied since the 70 s of the last century [4]. Since then many works have focused on this topic, mainly on the free-edge of a laminate because the modelization of a straight edge is simpler [5-8]. The stress ﬁeld around the hole is clearly three-dimensional and with large gradients in all the components [9,10]. Some works use analytical models [11,12] or numerical models [1,8] to estimate the three-dimensional stress ﬁeld in intact laminates. When damage appears, the stresses change and purely elastic models can not be considered valid. The analysis of open-hole laminates under compressive loads is important since the compressive strength in the direction of the ﬁbres is ⁎

Corresponding author. E-mail address: [email protected] (E. Barbero-Pozuelo).

https://doi.org/10.1016/j.compstruct.2019.03.027 Received 30 November 2018; Received in revised form 23 January 2019; Accepted 6 March 2019 Available online 07 March 2019 0263-8223/ © 2019 Elsevier Ltd. All rights reserved.

Composite Structures 217 (2019) 89–99

A. Solis, et al.

step t. Moreover, the outputs of this block are the composite σc , ﬁbre σf and matrix stresses σm needed for the internal forces calculation in the outer loop. S/PMT also produces the composite constitutive tensor C T needed for the global stiﬀness matrix K T calculation in the following outer loop iteration. From the ﬁbre [dεf ]q and matrix [dεm ]q strains, the explicit damage model calculates the ﬁbre [C f ]q and matrix [C m]q constitutive tensors and the stresses in each q iteration of the inner loop. S/PMT provides the composite constitutive tensor by combining ﬁbre, and matrix constitutive tensors and reduces, through successive iterations, the diﬀerence between ﬁbre and matrix serial stresses.

In a previous work, the authors analysed the edge eﬀect in laminates without damage subjected to tensile loads [8] due the symmetries of the stress ﬁeld of this problem some simpliﬁcation reduced the complexity of the model. To analyse laminates with holes and with damage more complex models are needed. The serial-parallel mixing theory (S/PMT) [36] is an alternative to other methodologies such as mesomechanical or micromechanical models. Some of these models require the estimation of a large number of parameters that are diﬃcult to measure experimentally. Mesomechanical models consider the material as a homogeneous continuous medium and have limitations for predicting ﬁbre and matrix failure separately. Micromechanical models are based on a detailed deﬁnition of the heterogeneity of the composite material and are extremely complex and diﬃcult to apply to structural problems [36]. As described by his authors, S/PMT combines speed and accuracy and is based on combining relatively simple constitutive equations for the constituents, ﬁbre and matrix, and at the same time is able to reproduce the anisotropy and heterogeneity of a laminate. This theory has been applied successfully to predict the fatigue behaviour [37] and the evolution of delamination [38] in laminates. S/ PMT has not been used to analyse the interlaminar stresses and damage initiation in problems with stress concentration. In this work, a phenomenological model was used by combining S/ PMT with a CDM to predict the interlaminar stresses near the free-edges and the hole-edge at the damage onset. The method proposed analysed the microbuckling eﬀect of the ﬁbres oriented according to the load direction, developed in two laminates with diﬀerent stacking sequences. This failure mode initiation was predicted thanks to the possibility of deﬁning diﬀerent threshold limits for tensile and compressive loads. This avoids the need for the micromechanical formulation developed in [39] regarding ﬁbre microbuckling or any other solution that includes the explicit complexity of the physics involved. The mentioned complexity is one of the main diﬃculties in compression problems as revealed in [16]. The model was calibrated using experimental data from unidirectional unnotched laminates and it was validated using the experimental results of multidirectional unnotched and notched laminates subjected to a compression load [40].

2.1. Serial/Parallel Mixing theory This theory is based on the following hypothesis:

• The composite material is made of two diﬀerent components, ﬁbre •

and matrix. The material is modelled as homogeneous with a perfect bond between the components, where the component participations are proportional to their volumetric fractions. The components exhibit a parallel behaviour in the ﬁbre direction (iso-strain) and a serial behaviour (iso-stress) in the perpendicular direction.

In this work, a separation between parallel and serial components was implemented by rearranging the components of the strain and stress vectors written according to Voigt notation. The reordering can be expressed by using a projection matrix P. The ε and ?? vectors are transformed into ε' and ??' where the parallel components are placed in the ﬁrst rows and then, the remaining serial components. In such a way:

εp σp ε ' = Pε = ⎛ ⎞; σ ' = Pσ = ⎛ ⎞ ⎝ σs ⎠ ⎝ εs ⎠

(1) ‘ jth ’

component in ε Each ‘ij’ element in the Pij (6x6) matrix is 1 if the or σ corresponds to the ‘ith ’ component of ε' or σ' and is 0 in any other case. P can be split into two matrices Pp and Ps . The ﬁrst n rows in Pp correspond to the ﬁrst n rows in P while the remaining rows contain null elements, with n the number of components with parallel behaviour. Complementarily, the last (6-n ) rows in Ps correspond to the last (6-n ) rows in P while the other n rows contain null elements. This can be expressed as:

2. Model description and validation In this work, a Continuum Damage Mechanics (CDM) model was used to simulate the damage initiation process due to ﬁbre microbuckling in laminates subjected to compressive loads. The Serial/ Parallel Mixing theory (S/PMT) [36] was applied to characterize the mechanical behaviour of a multidirectional laminate by combining the ﬁbre and matrix mechanical properties. The CDM model and S/PMT were implemented in an iterative ﬁnite element algorithm developed for non-linear problems in this work. A general scheme of the algorithm is summarized in Fig. 1. The algorithm is composed of two loops. An outer loop (with iteration index i) deﬁnes the equilibrium between internal and external forces in the Finite Element Method (FEM), and an inner loop (with iteration index q) that balances the iso-stress components according to the relations imposed by S/PMT. The outer loop inputs are the ﬁbre and matrix mechanical properties and damage parameters, all ply deﬁnition constants (volumetric fractions, directions with parallel behaviour and ﬁbre direction) and boundary conditions. Once convergence is reached, the outer loop produces as outputs, the nodal forces f and displacements u , and the strain and stress components of composite, ﬁbre and matrix (εc , εf , εm, σc , σf , σm) . For each Gauss point and element in the model, the inner loop uses a Newton-Raphson iterative scheme to obtain the strain and stress tensors of the composite that verify the iso-strain and iso-stress conditions required by the S/PMT. These block inputs are composite strains in the next time step [dε c ]ti + Δt and ﬁbre [dεf ]t and matrix strains [dεm ]t in the

P = Pp + Ps

(2)

In the model proposed, only the ﬁbre direction (in each ply local axis) acts according to a parallel behaviour so that n = 1 and the parallel components are εxx and σxx . The theory enables any constitutive law for the ﬁbre and matrix to be considered separately. In this work, given that ﬁbre microbuckling determines laminate failure, the ﬁbre was modelled according to a continuum isotropic damage model whereas the matrix was modelled as an elastic material. Under these conditions, ﬁbre and matrix constitutive laws are:

σf = (1 − df ) Cf εf ; σm = Cm εm

(3)

where Cf and Cm are the constitutive tensors of ﬁbre and matrix and df is the scalar damage ﬁbre variable. The serial/parallel decomposition described above can be applied in (3) by using the P matrix deﬁned in (1) and (2):

Cpp Cps ⎞ εp σp ⎞ ; i = f, m σi' = ⎛ ⎞ = (1 − di ) Ci' εi' = (1 − di ) ⎛⎜ ⎟ ⎛ ε C C ⎝ σs ⎠i ⎝ sp ss ⎠i ⎝ s ⎠i

(4)

where:

Ci' = (Pp Ci PpT + Pp Ci PsT + Ps Ci PpT + Ps Ci PsT ) Cpp (nxn) Cps (nx (6 − n)) ⎞ = ⎜⎛ ⎟ ; i = f, m C ((6 − n ) xn ) C ss ((6 − n ) x (6 − n )) ⎠ ⎝ sp i 90

(5)

Composite Structures 217 (2019) 89–99

A. Solis, et al.

Fig. 1. General scheme of the method.

the iteration q of the inner loop) can be cleared from the second equation of (6):

In (5), the submatrix dimensions are included in brackets. Given that the matrix behaves elastically, dm = 0 , while df is given by the continuum damage model described later. The relations between composite strains and stresses and ﬁbre and matrix strains and stresses are given by the usual rule of mixtures applied according to a parallel and serial decomposition as described in (1):

(σp )c = k f (σp )f + k m (σp )m

(parallel behaviour)

(εs )c = k f (εs )f + k m (εs )m

(serial behaviour)

[εs f ]tq+ Δt =

(σs )f = (σs )m = (σs )c

;

(parallel behaviour) (serial behaviour)

(6)

;

[Δσs ]q = [σs m]tq+ Δt − [σs f ]tq+ Δt ≤ tolerance

(7)

∂ (Δσs ) ⎤ km = [(Css )m ]q + f [(Css )f ]q Jq = ⎡ m ⎥ ⎢ ∂ ε k + m t Δ t ⎣ s ⎦[εs ]q

(11)

This Jacobian is inserted in a Newton-Raphson scheme that provides the next iteration value for the matrix serial strain.

[εs m]tq++Δ1t = [εs m]tq+ Δt − Jq−1 [Δσs ]q

(12)

In order to have quadratic convergence, the Jacobian described in (11) has to be calculated using the constitutive tangent tensors of the components. For the calculation of these tensors, the numerical derivation technique described in [38] is used. The composite constitutive tensor needs to be estimated when the inner loop converges. This tensor is required to calculate the global stiﬀness matrix in the iteration i in the outer loop. To obtain the

[(Δεs )m ]o = (k m (Css )f + k f (Css )m)−1 [(Css )f (Δεs )c

[εs m]to+ Δt

(10)

If [Δσs ]q is less than the tolerance deﬁned in (10), the strain–stress state is correct and the stress state of the composite can be calculated through the application of the inverse second equation of (1). Otherwise, the stress state has to be corrected with the Newton-Raphson method proposed by Rastellini et al. [36], where the initial approach is minimized using the Jacobian of the residual stresses. This Jacobian (in the iteration q of the inner loop) can be written as follows:

The S/PMT algorithm calculates the composite, ﬁbre and matrix stresses in the instant t + Δt from the composite strains at the instant t + Δt (obtained in the iteration i of the outer loop) and ﬁbre and matrix strains at the instant t. The ﬁrst step is the separation of strains and stresses in the serial and parallel components as described in (1). According to the ﬁrst equation in (7), composite, ﬁbre and matrix parallel strains are equal, however, serial strains are unknown and their calculation needs an initial approximation for either the matrix or the ﬁbre. Rastellini [41] proposed as an initial approximation for the increment of matrix serial strain:

+ k f ((Csp )f − (Csp )m )(Δεp )c ]

(9)

When parallel and serial components of ﬁbre and matrix strains are determined, these have to be rearranged (according to the original order of ε and σ ) to apply the constitutive law of each component given in (3). After this, the ﬁbre and matrix stresses are calculated and the serial components should verify:

where c, f and m respectively represent composite, ﬁbre and matrix and k f and k m are the volumetric fractions. The closure equations imposed by the theory can be expressed easily using the serial/parallel separation described in (1):

(εp )f = (εp )m = (εp )c

1 c t + Δt km [εs ] − f [εs m]tq+ Δt kf k

(8)

m]t .

where [(Δεs )m ]o = Constitutive tensors showed in (8) − [εs are the ﬁbre and matrix tangent constitutive tensors in the instant t, decomposed as described in (5). Once [εs m]tq+ Δt is determined, [εs f ]tq+ Δt (in 91

Composite Structures 217 (2019) 89–99

A. Solis, et al.

composite constitutive tensor from the ﬁbre and matrix constitutive tensors in their parallel and serial components the following relations were used [31]:

3

∑i = 1 〈σi 〉

r=

3

∑i = 1 |σi |

(20) 1 [x 2

+ |x|]. The where 〈x 〉 is the McAully function deﬁned as 〈x 〉 = weight function φ (r ) transforms the tensile loads into equivalent compressive loads being weighted by the tensile strength. With this approach, the damage threshold c (d ) and c max deﬁned in (15) and (16) must be deﬁned using the compression stress, while the diﬀerence between the compression and the tensile threshold is deﬁned by the parameter N, which is a property of the material. The evolution of the damage scalar variable d in softening behaviour can be deduced from the Kuhn-Tucker conditions. From the −̇ consistency condition F (σo, d ) = 0 , it can be demonstrated that [39]:

(Cpp )c = (k f (Cpp )f + k m (Cpp )m) + k f k m ((Cps )f − (Cps )m )(k m (Css )f + k f (Css )m)−1 ((Csp )m − (Csp )f ) (Cps )c = (k f (Cps )f (k m (Css )f + k f (Css )m)−1 (Css )m + k m (Cps )m (k m (Css )f + k f (Css )m)−1 (Css )f ) (Csp )c = (k m (Css )f (k m (Css )f + k f (Css )m)−1 (Csp )m + k f (Css )m (k m (Css )f + k f (Css )m)−1 (Csp )f )

d = G [f (σo)]

(21)

1

(Css )c = 2 ((Css )f (k m (Css )f + k f (Css )m)−1 (Css )m + (Css )m (k m (Css )f + k f (Css )m)−1 (Css )f )

The function that is proposed for G [f (σo)] takes the form: (13)

f (σ )

2.2. Damage model

A=

(14)

(23)

K l

(24)

The developed model was applied to estimate the response of a laminate plate with and without hole subjected to compressive loads. Specimens of 245 × 50 × 3 mm3 and 5 mm diameter centred hole were modelled. The plate was meshed by isoparametric, hexaedrical elements with eight nodes per element. The shape functions were linear and the quadrature rule for the integration of the local stiﬀness matrices was deﬁned on eight Gauss points. The laminate plate was clamped at one end and was subjected to a uniform compression load at the other end. The model was validated by experimental data of a carbon ﬁbre laminate T800/924C with two stacking sequences, unidirectional and [ ± 45/02]3S [40]. The mechanical properties were taken from the scientiﬁc literature [18,40]. To analyse the sensitivity of the results to the mesh size, four different meshes with 9600, 19968, 28,800 and 44,928 elements (Fig. 2) were used. The global response of the laminate was not aﬀected by the number of elements in the mesh (Fig. 3). However, near the hole, the stress ﬁeld

(17)

In this work, the Simo-Ju generalized criteria [43] is used as yield function f (σo) . This function can be written: (18)

In (18), φ (r ) is a weight function that describes the relations between the compression and tensile loads:

φ (r ) = rN + (1 − r )

1 2

2.3. Model calibration and validation

(16)

−

f (σo) = φ (r ) εCo ε

N2 −

where K is the energy (per unit area) release rate, Ac is the crack area and l is the damage length which is perpendicular to the aﬀected area. In a continuum material this length l tends to zero, however, if this formulation is applied to a ﬁnite element code, l takes a ﬁnite value. In the model proposed, l corresponds to the characteristic dimension of each ﬁnite element, which can be estimated by the cubic root of the element volume.

(15)

Particularly, instead of (15) the damage criteria is transformed into an equivalent form by using a monotonous increasing, semi-positive, invertible and scalar G function:

F (σo, d ) = G [f (σo)] − G [c (d )]

1 gf cmax2

gf V = gf Ac l = KAc → gf =

where c (d ) deﬁnes the damage threshold and f (σo) characterizes the yield surface. Damage starts to grow when f (σo) reaches c (d ) and, hence, F (σo, d ) goes to zero. F (σo, d ) keeps its null value as long as damage evolves. Before any damage level is reached, the value of c (d ) is associated with c max known as ﬁrst damage threshold and is updated according to:

c (d ) = max {c max , max {f (σo )}s}; 0 ≤ s ≤ t

(22)

where gf is the maximum energy (per unit volume) dissipated by the material under compressive loads. The connection between the described damage model and the Fracture Mechanics model is established by matching the dissipated energy and the required energy to open new surfaces:

where d is the scalar damage variable that is 0 when the material is intact and is 1 if the material is completely damaged. The eﬀective stress σo is calculated using the constitutive elastic law Co and the corresponding strain level ε . The degradation initiation and evolution process is described through a yielding function. Typically, this function adopts the form:

F (σo, d ) = f (σo) − c (d )

⎟

Eq. (22), formulated by Oliver et al. [44], proposes an exponential softening for the damage variable d. The parameter c max corresponds to the maximum compressive load in a compressive pure state. The parameter A shown in (22) is obtained from the dissipation material equation by considering a uniaxial monotonous increasing load process. The expression of the parameter A in these conditions according to Oller [45], is:

The material degradation process can be described using the Continuum Damage Mechanics model formulated by Kachanov [32]. In this work, microbuckling was modelled by a reduction of the stiﬀness and strength properties through a scalar damage variable that establishes the degradation level in each Gauss point. To simulate the constitutive law of the ﬁbre, the isotropic damage model deﬁned by Oller [42] was applied. This model deﬁnes diﬀerent thresholds for tensile and compression stresses. The degraded stress σ is obtained isotropically from the eﬀective stress σo through:

σ = (1 − d ) σo = (1 − d ) Co ε

c max A ⎛1 − maxo ⎞ e ⎝ c ⎠ f (σo ) ⎜

d = G (f (σo)) = 1 −

(19)

max σcomp

with N = σ max , the relation between the maximum compression and trac tensile loads and r is taken from [44] and deﬁnes the relations between the compression and tensile eigenvalues of the stress tensor: 92

Composite Structures 217 (2019) 89–99

A. Solis, et al.

Fig. 2. Meshes used in the sensitivity analysis. a) 9600 elements, b) 19,968 elements, c) 28,800 elements, d) 44,928 elements.

Fig. 4. Inﬂuence of the mesh size in the stress σxx vs. distance from hole-edge in transversal direction in a laminate [ ± 45/02]3s with a 5 mm diameter hole.

Fig. 3. Inﬂuence of the mesh size in the applied load–displacement curve in a laminate [ ± 45/02]3s with a 5 mm diameter hole.

93

Composite Structures 217 (2019) 89–99

A. Solis, et al.

3. Results In this section, a laminate plate with a centred hole of 5 mm in diameter subjected to a uniaxial compression load was studied using the proposed model. Two diﬀerent laminates, [45/−45/02]3?? and [902/02]3s of the material used in the previous section, were modelled. The interlaminar stresses that appear at the hole-edge and free-edges were analysed. In both laminates, the same strain level was applied. The results show that the model predicts the damage localization in both laminates. The damage initiates in the middle plane of the laminate where the thickest block of plies oriented in the load direction is located. Later, the damage progressively propagates to the nearest block of layers with the same orientation, to the top and bottom of the laminate (Fig. 7). This damage can be caused by ﬁbre microbuckling that appears in laminates subjected to compressive loads. The damage is higher in the [902/02]3?? laminate than in the [45/−45/02]3?? laminate, due to the fact that the plies at 0° support more applied load than the plies at 90°. The distributions of the interlaminar stresses around the hole are shown in Fig. 8 and Fig. 9 in the three plies of diﬀerent orientation furthest to the plane of the symmetry of the laminate. The compression load is applied from the right end of the laminate plate while the ﬁxed boundary condition is on the left end. In all the plies, the stresses in the quadrature points are represented. For this reason, the stresses in the upper ply are diﬀerent from zero. Figs. 8 and 9 show that a change in the stacking sequence modiﬁes the interlaminar stresses. In the [45/ −45/02]3?? laminate (Fig. 8), the stress σzz presents an axial symmetry around the Z-axis. In the [902/02]3s laminate, a symmetry with respect to the X and Y -axes also appears (Fig. 9). Soutis et al. [40] experimentally observed the appearance of warping in the laminate around the hole. In this work, the model reproduced that phenomenon. In both laminates, the stress σzz at the edge of the hole change from tensile to compression when the angular coordinate varies. Delamination could appear in areas with tensile stress σzz, although this failure mode was not explicitly modelled. The stress σxz presents axial antisymmetry with respect to the Z-axis in both laminates. In the [45/−45/02]3?? laminate, there is also symmetry with respect to the X-axis and antisymmetry with respect to the Y-axis in the ply at 0° nearest to the top surface. In the [902/02]3?? laminate, this behaviour also appears in the second ply at 90° of the sublaminate. The maximum shear stress σxz is twice as the stress σyz for all plies of both laminates. In both laminates, the stress σyz presents axial antisymmetry with respect to the Z-axis. In the [902/02]3?? laminate, all the plies present symmetry with respect to the Y-axis and antisymmetry with respect to

Fig. 5. Compressive stress–strain curve of the T800/924C unidirectional laminate. Experimental and numerical curve after calibration.

was diﬀerent for each mesh. In order to estimate appropriately the stress concentration phenomenon with a moderate computational cost, a mesh with 28,800 elements was selected (Fig. 4). The calibration was carried out using the experimental data corresponding to a unidirectional laminate subjected to uniaxial compression load [40]. In the S/PMT, the ﬁbre and matrix properties are considered belonging to a diﬀerent anisotropy space that can eventually become isotropic [46]. In this way, the mesoscopic behaviour of the ply is as observed in the experimental test so that equivalent properties for the constituents that allow reproduction of the experimental strain–stress curve are ﬁxed, (Fig. 5). This process provides equivalent properties for the constituents that allow the behaviour of an unnotched and notched laminate with a [± 45, 02]3s stacking sequence to be reproduced. An excellent correlation in stiﬀness and damage initiation prediction, between numerical and experimental results, was found (Fig. 6). Therefore, the proposed model can predict the damage due to ﬁbre microbuckling in open-hole laminates subjected to compressive loads. It enables modelling the orthotropic behaviour of multidirectional laminates without the use of second or fourth order damage tensors as proposed by other authors [34,35], which would increase the number of internal variables and the computational cost.

a)

b)

Fig. 6. Comparison of experimental and numerical compressive stress–strain curves a) unnotched [ ± 45/02]3s laminate, b) laminate [ ± 45/02]3s with a 5 mm diameter hole. 94

Composite Structures 217 (2019) 89–99

A. Solis, et al.

Fig. 7. Localization of ﬁbre damage initiation in 0° plies. Left: Laminate [45/−45/02]3?? Right: Laminate [902/02]3??

Fig. 8. Stresses σ??z, σx?? y σ???? (from left to right) for the plies with 45°, −45° and 0° orientations furthest to the plane of symmetry (from top to bottom). Laminate [45/−45/02]3??.

Fig. 9. Stresses σ??z, σx?? y σ???? (from left to right) for the plies with 90° and 0° orientations furthest to the plane of symmetry (from top to bottom). Laminate [902/ 02]3??. 95

Composite Structures 217 (2019) 89–99

A. Solis, et al.

Fig. 10. Location of the elements where the interlaminar stress components along the thickness are estimated: close to the hole-edge perpendicular to the load direction (location A1 and A2), in the load direction (location B) and at the free edge (location C).

the X-axis. This behaviour is the opposite to that observed for stress σxz. The areas of the diﬀerent plies, in which the highest interlaminar shear stresses appear, are the most susceptible to transverse shear failure. The maximum σxz is located at the hole-edge in the applied load direction for the two laminates analysed, and for the stress σyz, the maximum value point is placed at 90° from the load direction. The points at which these stresses are null are located at 90° from those corresponding to the maximum values. The evolution of the interlaminar stresses along the thickness in four locations was also analysed for the two laminates. Three of the locations correspond to elements located in the edge of the hole (locations A1, A2 and B) and the other to the free-edge (location C), Fig. 10. The locations A1, A2 and C are on the mid-line perpendicular to the load direction. The distance between location A1 and A2 is 2 mm and they are in the area of highest stress σxx. Location B corresponds to elements at the edge of the hole in the direction of application of the load, in which the interlaminar stress σxz is maximum. In both laminates, the stress σzz presents a symmetry with respect to the middle plane of the laminate (Fig. 11). By contrast, the stresses σxz and σyz present an antisymmetric distribution with respect to the same plane (Figs. 12 and 13). Figs. 11 and 12 show a high level of stress concentration in the interlaminar stress components at the hole-edge (locations A1, A2 and B) with respect to the free-edge of the laminate (location C). Tensile stress σzz is observed in the locations A2 and B (at the holeedge). For this reason, in these two areas, delamination damage can be produced. By contrast, in location A1, σzz is in compression and thus

delamination is restricted. In both laminates, the distribution of tensile stress in locations A2 and B is of the same order, with the compression stress (location A1) being higher in laminate [902/02]3??. The maximum stress σzz appears close to the plane of symmetry of the laminate where the largest block of plies at 0° (four plies) in both laminates is located. In laminate [45/−45/02]3s, small oscillations of this stress component appear in the ply interfaces; this phenomenon is not observed in the other laminate. Also, in the [45/−45/02]3s laminate, the distribution of the interlaminar shear stresses through the thickness presents oscillations in the interface between the plies. In the other laminate, these oscillations are much less ostensible. The shear stresses σxz and σyz show sign changes along the thickness in the ply interfaces in the [45/−45/02]3s laminate. This phenomenon can encourage transverse shear failure due to the shear displacement between plies. These changes of sign do not appear in the other laminate. The stress σxz in location B is greater than the stress σyz in both laminates, with the highest value being found in the ﬁrst of the laminates. By contrast, in location A1, the relative value of both shear stress components are the opposite, and in location A2 the two stress components are of the same order.

4. Conclusions The phenomenological model proposed in this work allows to obtain the interlaminar stresses at the hole-edge and free-edge of an openhole laminate subjected to in-plane compressive loads. The S/PMT with 96

Composite Structures 217 (2019) 89–99

A. Solis, et al.

Fig. 11. Stress σ??z distribution along laminate thickness. Left: Laminate [45/−45/02]3??. Right: Laminate [902/02]3??.

The model also can predict the inﬂuence of the stacking sequence on the interlaminar stresses that appear close to the hole. The distribution of the interlaminar stresses around the hole presented symmetry with respect to the load direction and the perpendicular axis. Values of interlaminar stresses with diﬀerent signs were found as the angular coordinate varied from 0° to 360°. The maximum and minimum values were located in diﬀerent angular positions for each stress component and laminate. The positions can be aligned with the axis of application of the load, the perpendicular axis or in points of angular coordinates at odd multiples of 45°. The alternate tensile and compressive values of the stress σzz around the hole reproduced the warping observed experimentally by other

an isotropic continuous damage model predicted damage initiation in compression, modelling the orthotropic behaviour of the laminate. In the laminates analysed, the damage initiated in the middle plane of the laminate, where the thickest block of plies oriented in the direction of the load is located. Subsequently, the damage progressively propagated to the closest block of plies with the same orientation to the top and bottom surface. This zone can be identiﬁed, therefore, with the area aﬀected by microbuckling, characteristic of the compression loads that are applied. These results show that is possible to characterize the damage by microbuckling with the proposed model, without using additional elements such as cohesive elements or mesh separation techniques, and thus reducing the computational cost.

Fig. 12. Stress σx?? distribution along laminate thickness. Left: Laminate [45/−45/02]3??. Right: Laminate [902/02]3??. 97

Composite Structures 217 (2019) 89–99

A. Solis, et al.

Fig. 13. Stress σy?? distribution along laminate thickness. Left: Laminate [45/−45/02]3s. Right: Laminate [902/02]3??. [14] Rosen BW. The tensile failure of ﬁbrous composites. AIAA J 1964;2(11):1885–911. [15] Barbero EJ. Prediction of compression strength of unidirectional polymer matrix composites. J Compos Mater 1998;5(32):483–502. [16] Su ZC, Tay TE, Ridha M, Chen BY. Progressive damage modeling of open-hole composite laminates under compression. Compos Struct 2015;122:507–17. [17] Wisnom MR, Hallet SR, Soutis C. Scaling eﬀects in notched composites. J Compos Mater 2010;44(2):195–209. [18] Soutis C, Curtis PT, Fleck NA. Static compression failure of notched carbon ﬁbre composite. Proceed: Mathemat Phys Sci 1901;1993(440):241–56. [19] Waas AM, Babcock CD, Query J, Knauss WG. An experimental study of compression failure of ﬁbrous laminated composites in the presence of stress concentration. Int J Sol Struct 1990;26(9/10):1071–98. [20] Moure MM, García-Castillo SK, Sanchez-Saez S, Barbero E, Barbero EJ. Inﬂuence of ply cluster thickness and location on matrix cracking evolution in open-hole composite laminates. Compos Part B – Eng 2016;95:40–7. [21] Green BG, Wisnom MR, Hallett SR. An experimental investigation into the tensile strength scaling of notched composites. Compos Part A – Appl S 2007;38:867–78. [22] Hallett SR, Green BG, Jiang WG, Wisnom MR. An experimental and numerical investigation into the damage mechanisms in notched composites. Compos Part A – Appl S 2009;40:613–24. [23] Chen BY, Tay TE, Baiz PM, Pinho ST. Numerical analysis of size eﬀects on open-hole tensile composite laminates. Compos Part A – Appl S 2013;47:52–62. [24] Leopold C, Schütt M, Liebig WV, Philipkowski T, Kürten J, Schulte K, et al. Compression fracture of CFRP laminates containing stress intensiﬁcations. Materials 2017;10:1039. [25] Whitney J, Nuismer R. Stress fracture criteria for laminated composites containing stress-concentrations. J Compos Mater 1974;8:253–65. [26] Chen P, Shen Z, Wang JY. Prediction of the strength of notched ﬁber-dominated composite laminates. Compos Sci Technol 2001;61(9):1311–21. [27] Camanho PP, Erçin GH, Catalanotti G, Mahdi S, Linde P. A ﬁnite fracture mechanics model for the prediction of the open-hole strength of composite laminates. Compos Part A – Appl S 2012;43(8):1219–25. [28] Dugdale D. Yielding of steel sheets containing slits. J Mech Phys Solids 1960;8(2):100–4. [29] Barbero EJ, Cortes DH. A mechanistic model for transverse damage initiation, evolution, and stifness reduction in laminated composites. Compos Part B – Eng 2010;41:124–32. [30] Moure MM, Otero F, Garcia-Castillo SK, Sanchez-Saez S, Barbero E, Barbero EJ. Damage evolution in open-hole laminated composite plates subjected to in-plane loads. Compos Struct 2015;133:1048–57. [31] Chaboche J-L. A continuum damage theory with anisotropic and unilateral damage. Rech Aeros 1995;2:139–47. [32] Kachanov L. Introduction to continuum damage mechanics. Netherlands: Springer; 1986. [33] Barbero EJ, De Vivo L. A constitutive model for elastic damage in ﬁber-reinforced PMC laminae. Int J Damage Mech 2001;10:73–93. [34] Maimí P, Camanho PP, Mayugo JA, Dávila CG. A continuum damage model for composite laminates: Part I – Constitutive model. Mech Mater 2007;39:897–908. [35] Wang L, Zheng C, Luo H, Wei S, Wei Z. Continuum damage modeling and

authors. In this area, delamination damage could appear. Acknowledgement The authors thank the funds received for the development of this work from Ministry of Economy and Finance of Spain within the framework of the project DPI2013-42240-R Appendix A. Supplementary data Supplementary data to this article can be found online at https:// doi.org/10.1016/j.compstruct.2019.03.027. References [1] Hu FZ, Soutis C, Edge EC. Interlaminar stresses in composite laminates with a circular hole. Compos Struct 1997;37:223–32. [2] Sun CT, Chu GD. Reducing free edge eﬀect on laminate strength by edge modiﬁcation. J Compos Mater 1991;25(2):142–61. [3] Sihn S, Kim RY, Kawabe K, Tsai SW. Experimental studies of thin-ply laminated composites. Compos Sci Technol 2007;67(6):996–1008. [4] Pipes RB. Moiré analysis of the interlaminar shear edge eﬀect in laminated composites. J Compos Mater 1971;5:253–69. [5] Islam MS, Prabhakar P. Modeling framework for free edge eﬀects in laminates under thermomechanical loading. Compos B 2017;116:89–98. [6] Dhanesh N, Kapuria S, Achary GGS. Accurate prediction of three-dimensional free edge stress ﬁeld in composite laminates using mixed-ﬁeld multiterm extended Kantorovich method. Acta Mech 2017;228:2895–919. [7] Hajikazemi M, Van Paepegem W. A variational model for free-edge interlaminar stress analysis in general symmetric and thin-ply composite laminates. Compos Struct 2018;184:443–51. [8] Solis A, Sánchez-Sáez S, Barbero E. Inﬂuence of ply orientation on free-edge eﬀects in laminates subjected to in-plane loads. Compos Part B – Eng 2018;153:149–58. [9] Suemasu H, Naito Y, Gozu K, Aoki Y. Damage initiation and growth in composite laminates during open hole compression tests. Adv Compos Mater 2012;21(3):209–20. [10] Suemasu H, Takahashi H, Ishikawa T. On failure mechanisms of composite laminates with an open hole subjected to compressive load. Compos Sci Technol 2006;66:634–41. [11] Ko CC, Lin CC. Method for calculating the interlaminar stresses in symmetric laminates containing a circular hole. AIAA J 1992;30(1):197–204. [12] Iarve EV, Pagano NJ. Singular full-ﬁeld stresses in composite laminates with an open hole. Int J Solids Struct 2001;38:1–28. [13] Hahn HT, Willianms, JG. Compression failure mechanisms in unidirectional composites. NASA Technical Memorandum 85834; 1984.

98

Composite Structures 217 (2019) 89–99

A. Solis, et al.

[36]

[37]

[38]

[39] [40]

progressive failure analysis of carbon ﬁber/epoxy composite pressure vessel. Compos Struct 2015;134:475–82. Rastellini F, Oller S, Salomon O, Oñate E. Composite materials non-linear modelling for long ﬁbre reinforced laminates: continuum basis, computational aspects and validations. Comput Struct 2008;86(9):879–96. Salomon O, Rastellini F, Oller S, Oñate E. Fatigue prediction for composite materials and structures. In: Symposium on the evaluation, control and prevention of high cycle fatigue. Granada, Spain; 2005. Martinez X, Oller S, Barbero E. Caracterización de la delaminación en materiales compuestos mediante la teoría de mezclas serie/paralelo. Revista Internacional de Métodos Numéricos para Cálculo y Diseño en Ingeniería 2010;3(27):192–3. Martinez X, Oller S. Numerical simulation of matrix reinforced composite materials subjected to compression loads. Arch Comput Method E 2009;16(4):357–97. Soutis C, Fleck NA, Curtis PT. Hole-hole interaction in carbon ﬁbre/epoxy laminates

under uniaxial compression. Composites 1991;22(1):31–8. [41] Rastellini F. Modelización Numérica de la No-Linealidad Constitutiva de Laminados Compuestos. PhD thesis (In spanish). Polytechnic. Barcelona: University of Catalonia (UPC); 2006. [42] Oller S. Fractura mecánica. Un enfoque global. Publicaciones CIMNE; 2001. [43] Simo JC, Ju JW. Strain and stress-based continuum damage models-I. Formulation. Int J Solids Struct 1987;23(7):821–40. [44] Oliver J, Cervera M, Oller S, Lubliner J. Isotropic damage models and smeared crack analysis of concrete. In: Second International Conference on Computer Aided Analysis and Design of Concrete Structures. Austria; 1990. [45] Oller S. Dinámica No Lineal. Publicaciones CIMNE; 2001. [46] Oller S. Simulación Numérica del Comportamiento Mecánico de los Materiales Compuestos. Publicaciones CIMNE; 2003.

99

Copyright © 2024 C.COEK.INFO. All rights reserved.